Causes, Evaluation, and Repair of Cracks in Concrete StructuresReported by ACI Committee 224Robert J. Frosch* Chair Mohamed N. Abou-Zeid James P. Barlow* Florian G. Barth J. Floyd Best David Darwin John F. Duntemann* Member of task group that prepared these revisions. Chair of task group that prepared these revisions.
Jeffrey S. West Secretary Ralf Leistikow Peter A. Lipphardt Edward G. Nawy Kamran M. Nemati Keith A. Pashina Randall W. Poston Royce J. Rhoads John W. Roberts Andrew Scanlon Andrea J. Schokker
Fouad H. Fouad David W. Fowler Grant T. Halvorsen Will Hansen Harvey H. Haynes*
The causes of cracks in concrete structures are summarized. The procedures used to evaluate cracking in concrete and the principal techniques for the repair of cracks are presented. The key methods of crack repair are discussed, and guidance is provided for their proper application. Keywords: alkali-silica reaction; alkali-carbonate reaction; autogenous healing; concrete; consolidation; corrosion; cracking (fracturing); drying shrinkage; epoxy resins; evaluation; grouting; heat of hydration; mass concrete; methacrylates; mixture proportion; overlay; plastic; polymer; precast concrete; prestressed concrete; reinforced concrete; repair; resins; settlement shrinkage; shrinkage; slab-on-ground; specification; thermal expansion; volume change.
Chapter 2Evaluation of cracking, p. 224.1R-9 2.1Introduction 2.2Determination of location and extent of concrete cracking 2.3Selection of repair procedures Chapter 3Methods of crack repair, p. 224.1R-13 3.1Introduction 3.2Epoxy injection 3.3Routing and sealing 3.4Near-surface reinforcing and pinning 3.5Additional reinforcement 3.6Drilling and plugging 3.7Gravity filling 3.8Grouting 3.9Drypacking 3.10Crack arrest 3.11Polymer impregnation 3.12Overlay and surface treatments 3.13Autogenous healing Chapter 4References, p. 224.1R-18 4.1Referenced standards and reports 4.2Cited referencesACI 224.1R-07 supersedes ACI 224.1R-93 and was adopted and published in March 2007. Copyright 2007, American Concrete Institute. All rights reserved including rights of reproduction and use in any form or by any means, including the making of copies by any photo process, or by electronic or mechanical device, printed, written, or oral, or recording for sound or visual reproduction or for use in any knowledge or retrieval system or device, unless permission in writing is obtained from the copyright proprietors.
CONTENTS Preface, p. 224.1R-2 Chapter 1Causes and control of cracking, p. 224.1R-2 1.1Introduction 1.2Cracking of plastic concrete 1.3Cracking of hardened concreteACI Committee Reports, Guides, Standard Practices, and Commentaries are intended for guidance in planning, designing, executing, and inspecting construction. This document is intended for the use of individuals who are competent to evaluate the significance and limitations of its content and recommendations and who will accept responsibility for the application of the material it contains. The American Concrete Institute disclaims any and all responsibility for the stated principles. The Institute shall not be liable for any loss or damage arising therefrom. Reference to this document shall not be made in contract documents. If items found in this document are desired by the Architect/Engineer to be a part of the contract documents, they shall be restated in mandatory language for incorporation by the Architect/Engineer.
CONCRETE REPAIR MANUAL
PREFACE Cracks in concrete have many causes. They may affect appearance only, or they may indicate significant structural distress or a lack of durability. Cracks may represent the total extent of the damage, or they may point to problems of greater magnitude. Their significance depends on the type of structure, as well as the nature of the cracking. For example, cracks that are acceptable for buildings may not be acceptable in water-retaining structures. Good crack repair techniques depend on knowing the causes and selecting appropriate repair procedures that take these causes into account; otherwise, the repair may only be temporary. Successful long-term repair procedures must address the causes of the cracks as well as the cracks themselves. This report is intended to serve as a tool in the process of crack evaluation and repair of concrete structures. The causes of cracks in concrete are summarized along with the principal procedures used for crack control. Both plastic and hardened concrete are considered. The importance of design, detailing, construction procedures, concrete proportioning, and material properties are discussed. The techniques and methodology for crack evaluation are described. The need to determine the causes of cracking as a necessary prerequisite to repair is emphasized. The selection of successful repair techniques should consider the causes of cracking, whether the cracks are active or dormant, and the need for repair. Criteria for the selection of crack repair procedures are based on the desired outcome. Twelve methods of crack repair are presented, including the techniques, advantages and disadvantages, and areas of application for each. CHAPTER 1CAUSES AND CONTROL OF CRACKING 1.1Introduction This chapter presents a brief summary of the causes of cracks and means for their control. Cracks are categorized as occurring either in plastic concrete or hardened concrete (Kelly 1981; Price 1982). In addition to the information provided herein, further details are presented in ACI 224R and articles by Carlson et al. (1979), Kelly (1981), Price (1982), and Abdun-Nur (1983). Additional references are cited throughout the chapter. 1.2Cracking of plastic concrete 1.2.1 Plastic shrinkage crackingWhen moisture evaporates from the surface of freshly placed concrete faster than it is replaced by bleed water, the surface concrete shrinks. Due to the restraint provided by the concrete below the drying surface layer, tensile stresses develop in the weak, stiffening plastic concrete. This results in shallow cracks of varying depths that may form a random, polygonal pattern, or be essentially parallel to one another (Fig. 1.1). These cracks may be fairly wide (as much as 1/8 in. [3 mm]) at the surface. They range from a few inches to many feet in length, and are spaced from a few inches (millimeters) to as much as 10 ft (3 m) apart. Plastic shrinkage cracks begin as shallow cracks, but can become full-depth cracks later in the life of the concrete.
Fig. 1.1Typical plastic shrinkage cracking (Price 1982). Plastic shrinkage cracking is usually associated with the rapid loss of moisture caused by a combination of factors that include high air and concrete temperatures, low relative humidity, and high wind velocity at the surface of the concrete. Concrete with lower amounts of bleed water, such as those containing mineral admixtures (especially silica fume) have a greater tendency to undergo plastic shrinkage cracking than concrete with a greater tendency to bleed. Because plastic shrinkage cracking is due to a differential volume change in the plastic concrete, successful control measures require a reduction in the relative volume change between the surface and other portions of the concrete. Steps can be taken to prevent rapid moisture loss due to hot weather and dry winds (ACI 224R, 302.1R, and 305R). These measures include the use of fog nozzles to saturate the air above the surface and the use of plastic sheeting to cover the surface between finishing operations. Windbreaks to reduce the wind velocity and sunshades to reduce the surface temperature are also helpful. It is good practice to schedule flatwork after the windbreaks have been erected. During hot, windy weather with low humidity, it is sometimes advisable to reschedule the concrete placement or to initiate concrete operations at night. 1.2.2 Settlement crackingConcrete has a tendency to continue to consolidate after initial placement, vibration, and finishing. During this period, the plastic concrete may be locally restrained by reinforcing steel, a previous concrete placement, or formwork. This local restraint may result in voids, cracks, or both, adjacent to the restraining element (Fig. 1.2). When associated with reinforcing steel, settlement cracking increases with increasing bar size, increasing slump, and decreasing cover (Dakhil et al. 1975); this is shown in Fig. 1.3 for a limited range of these variables. The degree of settlement cracking may be intensified by insufficient vibration or by the use of leaking or highly flexible forms. Suprenant and Malisch (1999) demonstrated that the addition of fibers can reduce the formation of settlement cracks. The following items will reduce settlement cracking: Form design following ACI 347; Concrete vibration (and revibration) (ACI 309R); Provision of a time interval between the placement of concrete in columns or deep beams and the placement of concrete in slabs and beams (ACI 309.2R);
CAUSES, EVALUATION, AND REPAIR OF CRACKS IN CONCRETE STRUCTURES Use of the lowest possible slump; An increase in concrete cover; and Addition of fibers.
1.3Cracking of hardened concrete 1.3.1 Drying shrinkageA common cause of cracking in concrete is restrained drying shrinkage. Drying shrinkage is caused by the loss of moisture from the cement paste constituent, which can shrink by as much as 1%. Fortunately, aggregate particles provide internal restraint that reduces the magnitude of this volume change to about 0.06%. On the other hand, concrete tends to expand when wetted (the volume increase can be the same order of magnitude as that observed due to shrinkage). These moisture-induced volume changes are a characteristic of concrete. If the shrinkage of concrete could take place without restraint, the concrete would not crack. It is the combination of shrinka